| ||Format||Pages||Price|| |
|8||$50.00||  ADD TO CART|
|Hardcopy (shipping and handling)||8||$50.00||  ADD TO CART|
|Standard + Redline PDF Bundle||16||$60.00||  ADD TO CART|
Significance and Use
5.1 The melting temperature range of a compound broadens as the impurity level rises. This phenomenon is described approximately by the van’t Hoff equation for melting point depressions. Measuring and recording the instantaneous heat flow into the specimen as a function of temperature during such a melting process is a practical way for the generation of data suitable for analysis by the van’t Hoff equation.
5.2 The results obtained include: sample purity (expressed as mole percent); enthalpy of fusion (expressed as J/mol); and the melting temperature (expressed in Kelvin) of the pure form of the major component.
5.3 Generally, the repeatability of this test method decreases as the purity level decreases. This test method is ordinarily considered unreliable when the purity level of the major component of the mixture is less than 98.5 mol % or when the incremental enthalpy correction (c) exceeds 20 % of the original detected enthalpy of fusion.
5.4 This test method is used for quality control, specification acceptance, and research.
1.1 This test method describes the determination of purity of materials greater than 98.5 mole percent purity using differential scanning calorimetry and the van’t Hoff equation.
1.2 This test method is applicable to thermally stable compounds with well-defined melting temperatures.
1.3 Determination of purity by this test method is only applicable when the impurity dissolves in the melt and is insoluble in the crystal.
1.4 The values stated in SI units are to be regarded as standard. No other units of measurement are included in this standard.
1.5 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety, health, and environmental practices and determine the applicability of regulatory limitations prior to use.
1.6 This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
E473 Terminology Relating to Thermal Analysis and Rheology
E793 Test Method for Enthalpies of Fusion and Crystallization by Differential Scanning Calorimetry
E794 Test Method for Melting And Crystallization Temperatures By Thermal Analysis
E967 Test Method for Temperature Calibration of Differential Scanning Calorimeters and Differential Thermal Analyzers
E968 Practice for Heat Flow Calibration of Differential Scanning Calorimeters
E1970 Practice for Statistical Treatment of Thermoanalytical Data
E2161 Terminology Relating to Performance Validation in Thermal Analysis and Rheology
ICS Number Code 17.200.10 (Heat. Calorimetry)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM E928-19, Standard Test Method for Purity by Differential Scanning Calorimetry, ASTM International, West Conshohocken, PA, 2019, www.astm.orgBack to Top